Effect of TiO2 rutile nanorods on the photoelectrodes of dye-sensitized solar cells
© Jung et al.; licensee Springer. 2013
Received: 25 November 2012
Accepted: 29 December 2012
Published: 19 January 2013
In order to enhance the electron transport on the photoelectrodes of dye-sensitized solar cells, one-dimensional rutile nanorods were prepared using electrospun TiO2 nanofibers. The grain size of the nanorods increased with increasing temperature. Electrochemical impedance spectroscopy measurements revealed reduced interface resistance of the cells with the one-dimensional rutile nanorods due to the improved electron transport and the enhanced electrolyte penetration. Intensity-modulated photocurrent/photovoltage spectroscopy showed that the one-dimensional rutile nanorods provided the electrons with a moving pathway and suppressed the recombination of photogenerated electrons. However, an excessive quantity of rutile nanorods created an obstacle to the electrons moving in the TiO2 thin film. The photoelectrode with 7 wt.% rutile nanorods optimized the performance of the dye-sensitized solar cells.
KeywordsOne-dimensional TiO2 nanorods Photoelectrode Electron transfer Dye-sensitized solar cells
One-dimensional (1-D) structured TiO2 nanorods show improved electrical and optical properties in the photoelectrodes of dye-sensitized solar cells (DSSCs). They can provide straight moving paths for electrons and reduce the e−/h+ recombination[2–4]. Further, they scatter sunlight so that the incident light stays longer in the cell. As these properties enhance the solar energy conversion efficiency, much research into the effects of the 1-D structured TiO2 on the photoelectrode have been conducted[6–8].
In principle, photoexcited electrons from dye molecules move on a TiO2 nanocrystal undergoing a series of trapping and de-trapping events during diffusion. The 1-D nanorods, which are densely packed TiO2 nanoparticles, could act as a single crystal and be involved in rapid electron transport, thereby reducing the chances for electron recombination. Furthermore, the TiO2 film with random packing of 1-D rods helps the electrolyte to penetrate into the photoelectrode because of the porosity[9, 10]. The enhanced interpenetration of electrolyte leads to the dye regeneration by redox process of the electrolyte and enhances the energy conversion efficiency with improved photocurrent.
Few grain boundaries in the TiO2 nanorods induce fast electron transport and decrease the electron recombination due to the reduced number of trapping sites in the interfaces. In order to reduce grain boundaries in the nanorods, the crystal size should be increased. TiO2 crystal structure (anatase and rutile) and size can be controlled by sintering temperature. The anatase phase has been reported to be developed at temperatures below 800°C, and above the temperatures, it transforms to the more stable rutile phase. Also, the TiO2 nanorods sintered at a high temperature have high crystallinity, meaning reduced grain boundaries and decreased trap sites. Electrons moving through the rutile structure undergo less stress because of the reduced number of trap sites on the grain boundaries[13, 14]. In addition, the transported electrons can easily migrate from the rutile to anatase phase[15, 16]. As the conduction band of the pure anatase phase is typically 0.2 eV more negative than that of the rutile phase, photoexcited electrons injected into the rutile phase migrate to the conduction band of the anatase phase, before passing through the external circuit. The resulting synergistic effects between the anatase and rutile phases lead to energetic electron flows and enhanced photocurrents[17–19].
However, even though the rutile 1-D nanorods provide the electrons with a better moving path and improve electrolyte penetration, a large number of rutile phases simultaneously can become a barrier for electron transport. The increased amount of rutile phase increases the probability of the moving electrons facing a higher energy level, which increases the internal resistance.
In this study, in order to make photoelectrodes with the 1-D rutile nanorods, the electrospun TiO2 nanofibers were sintered at various temperatures. The photoelectrodes considerably improved the DSSC energy conversion efficiency, depending on the amount of TiO2 nanorods. The intensity-modulated photocurrent spectroscopy, intensity-modulated photovoltage spectroscopy, charge-transfer resistance, and I-V characteristics of the DSSCs were investigated in order to study the effects of the rutile TiO2 nanorods on the cell performance. The purpose of this study is to investigate the effects of the crystal size and amount of the rutile TiO2 nanorods on the electron transport in the photoelectrodes of dye-sensitized solar cells.
Preparation of electrospun nanorods
Three grams of polyvinylpyrrolidone (PVP K90, MW = 130,000) was dissolved in 27 g of ethanol (Daejung Chemical & Metal Co., Ltd., Shiheung, South Korea), while the TiO2 precursor was prepared by adding 12 ml of acetic acid (Kanto Chemical Co., In., Tokyo, Japan) and 12 ml of ethanol into 6 ml of titanium(IV) isopropoxide (Junsei Chemical Co., Ltd., Tokyo, Japan), successively. The solutions were mixed and stirred for 12 h to obtain homogeneity. The solution was loaded into a syringe (SGE Analytical Science, Ringwood, Victoria, Australia) under an applied voltage of 9 kV. TiO2 nanofibers were electrospun on Al foil. The spinning rate was controlled by a syringe pump (KDS-100, KD Scientific, Holliston, MA, USA) at 2 ml/h. The tip-to-collector distance was maintained at 20 cm. The obtained TiO2 nanofibers were calcined at 450°C, 650°C, 750°C, 850°C, and 1,000°C.
Transmission electron microscopy (TEM) was used to examine the TiO2 nanorods, and the crystal structures were characterized by X-ray diffraction (XRD).
Fabrication of DSSCs with the TiO2 nanorods
The ground nanorods, sintered at 450°C, 650°C, 750°C, 850°C, and 1,000°C, were mixed into a homemade TiO2 (P25, Degussa-Hüls, Frankfurt/Main, Germany) paste at a loading of 3 wt.% as a preliminary experiment in order to choose the best nanorod. The ground nanorods sintered at 850°C were chosen and mixed into a commercial TiO2 anatase paste (Dyesol, Queanbeyan, New South Wales in Australia) at ratios of 0, 3, 5, 7, 10, and 15 wt.%. The TiO2 paste with the electrospun nanorods was cast on pre-cleaned fluorine-doped tin dioxide (FTO; Pilkington TEC glass, 8 Ω cm−2, Pilkington Group Limited, St Helens, UK) using a squeeze printing method. The TiO2 films were sintered at 450°C for 30 min. The thickness of the TiO2 films was about 10 μm, and the active area of the TiO2 electrode was 0.25 cm2. The obtained TiO2 film was immersed in 0.5 mmol ethanol solution of N719 dye (Solaronix, Aubonne, Switzerland) for 24 h to adsorb the dye molecules. A Pt counter electrode was fabricated by squeeze printing of the Pt-Sol (Solaronix) on an FTO substrate. The sandwich-type solar cell was assembled by placing a Pt counter electrode on the dye-sensitized TiO2 electrode. The redox electrolyte (Dyesol) was injected between the electrodes.
An AM 1.5 solar simulator (white light from a 150-W Xenon lamp, McScience, Suwon-si, South Korea) was used as the light source. The incident light intensity was calibrated with a standard Si solar cell (Japan Quality Assurance Organization, Tokyo, Japan). Electrochemical impedance spectroscopy (EIS) was conducted using Iviumstat (Ivium Technologies B.V., Eindhoven, the Netherlands) at an open-circuit potential at frequencies ranging from 10−1 to 105 Hz with an AC amplitude of 10 mV. The diffusion coefficients and electron lifetime of the electrons in the TiO2 films were determined using ModuLight-module under a red LED (λ = 625 nm) as light source (Ivium Technologies). The values of the diffusion coefficient and electron lifetime were obtained under 0.55-, 0.7-, 0.85-, and 1-V light intensity.
Results and discussion
Diffusion coefficients and lifetime values of the DSSCs with 1-D rutile nanorods at 1-V light intensity
Diffusion coefficient (cm2 s−1)
Lifetime (τr) (ms)
Cell performances of the DSSCs with the 1-D rutile nanorods
1-D rutile nanorods can provide a fast moving pathway for electrons and decrease electron recombination. In this study, the nanorods with high crystallinity showed enhanced energy conversion efficiency with reduced TiO2/electrolyte interface resistance. However, an excessive amount of randomly distributed rutile nanorods could create an obstacle to the moving electrons and reduce the internal surface area, even though they provided the electron moving paths. The charge-transfer resistance was decreased with increasing rutile nanorod loading up to 7 wt.%, but the electrical resistance was increased as the loading exceeded 10 wt.%. A 7 wt.% loading of 1-D rutile nanorods was considered the best condition for optimizing the performance of the DSSCs. The energy conversion efficiency of the optimized cell was 6.16%.
dye-sensitized solar cells
electrochemical impedance spectroscopy
fluorine-doped tin dioxide
transmission electron microscopy
This work was supported by the Priority Research Centers Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science and Technology (2009–0094055).
- Cozzoli PD, Kornowski A, Weller H: Low-temperature synthesis of soluble and processable organic-capped anatase TiO2 nanorods. J Am Chem Soc 2003, 125: 14539–14548. 10.1021/ja036505hView Article
- Ramakrishna S, Jose R, Archana PS, Nair AS, Balamurugan R, Venugopal J, Teo WE: Science and engineering of electrospun nanofibers for advances in clean energy, water filtration, and regenerative medicine. J Mater Sci 2010, 45: 6283–6312. 10.1007/s10853-010-4509-1View Article
- Manna L, Scher EC, Li LS, Alivisatos AP: Epitaxial growth and photochemical annealing of graded CdS/ZnS shells on colloidal CdSe nanorods. J Am Chem Soc 2002, 124: 7136–7145. 10.1021/ja025946iView Article
- Enache-Pommer E, Boercker JE, Aydil ES: Electron transport and recombination in polycrystalline TiO2 nanowire dye-sensitized solar cells. Appl Phys Lett 2007, 91: 123116–1-3.View Article
- Cuangchote S, Sgawa T, Yoshikawa S: Efficient dye-sensitized solar cells using electrospun TiO2 nanofibers as a light harvesting layer. Appl Phys Lett 2008, 93: 033310–1-3.
- Song MY, Kim DK: New application of electrospun TiO2 electrode to solid-state dye-sensitized solar cells. Synth Met 2005, 153: 77–80. 10.1016/j.synthmet.2005.07.129View Article
- Fujihara K, Kumar A, Jose R, Ramakrishna S, Uchida S: Spray deposition of electrospun TiO2 nanorods for dye-sensitized solar cell. Nanotechnology 2007, 18: 365709. 10.1088/0957-4484/18/36/365709View Article
- Thavasi V, Renugopalakrishnan V, Jose R, Ramakrishna S: Controlled electron injection and transport at materials interfaces in dye sensitized solar cells. Mater Sci Eng 2009, 63: 81–99. 10.1016/j.mser.2008.09.001View Article
- Park NG, van de Lagemaat J, Frank AJ: Comparison of dye-sensitized rutile- and anatase-based TiO2 solar cells. J Phys Chem B 2000, 104: 8989–8994.View Article
- Jiu JT, Isoda S, Wang F, Adachi M: Dye-sensitized solar cells based on a single-crystalline TiO2 nanorod film. J Phys Chem B 2006, 110: 2087–2092. 10.1021/jp055824nView Article
- Berger T, Teresa LV, Damian MS, Gomez R: An electrochemical study on the nature of trap states in nanocrystalline rutile thin films. J Phys Chem C 2007, 111: 9936–9942. 10.1021/jp071438pView Article
- Sen S, Mahanty S, Roy S, Heintz O, Bourgeois S, Chaumont D: Investigation on sol–gel synthesized Ag-doped TiO2 cermet thin films. Thin Solid Films 2005, 474: 245–249. 10.1016/j.tsf.2004.04.004View Article
- Lee KM, Suryanarayanan V, Ho K-C: A study on the electron transport properties of TiO2 electrodes in dye-sensitized solar cells. Sol Energ Mater Sol Cells 2007, 91: 1416–1420. 10.1016/j.solmat.2007.03.007View Article
- Lee BH, Song MY: Charge transport characteristics of high efficiency dye-sensitized solar cells based on electrospun TiO2 nanorod photoelectrodes. J Phys Chem C 2009, 113: 21453–21457. 10.1021/jp907855xView Article
- Hurum DC, Agrios AG, Gray KA, Rajh T, Thurnauer MC: Explaining the enhanced photocatalytic activity of Degussa P25 mixed-phase TiO2 using EPR. J Phys Chem B 2003, 107: 4545–4549. 10.1021/jp0273934View Article
- Leytner S, Hupp JT: Evaluation of the energetics of electron trap states at the nanocrystalline titanium dioxide/aqueous solution interface via time-resolved photoacoustic spectroscopy. Chem Phys Lett 2000, 330: 231–236. 10.1016/S0009-2614(00)01112-XView Article
- Li GH, Richter CP, Brudvig GW, Batista VS: Synergistic effect between anatase and rutile TiO2 nanoparticles in dye-sensitized solar cells. Dalton Trans 2009, 10078–10085.
- Barbe CJ, Arendse F, Comte P, Jirousek M, Lenzmann F, Shklover V, Gratzel M: Nanocrystalline titanium oxide electrodes for photovoltaic applications. J Am Ceram Soc 1997, 80: 3157–3171.View Article
- Kang SH, Choi SH, Kang MS, Kim JY, Kim HS, Hyeon TG, Sung YE: Nanorod-based dye-sensitized solar cells with improved charge collection efficiency. Adv Mater 2008, 20: 54–58. 10.1002/adma.200701819View Article
- Nakade S, Saito Y, Kubo W, Kanzaki T, Kitamura T, Wada Y, Yanagida S: Enhancement of electron transport in nano-porous TiO2 electrodes by dye adsorption. Electrochem Commun 2003, 5: 804–808. 10.1016/j.elecom.2003.07.008View Article
- Park KH, Hong CK: Morphology and photoelectrochemical properties of TiO2 electrodes prepared using functionalized plant oil binders. Electrochem Commun 2008, 10: 1187–1190. 10.1016/j.elecom.2008.05.046View Article
- Kang SH, Kim JY, Kim HS, Koh HD, Lee JS, Sung YE: Influence of light scattering particles in the TiO2 photoelectrode for solid-state dye-sensitized solar cell. J Photochem Photobio A: Chem 2008, 200: 294–300. 10.1016/j.jphotochem.2008.08.010View Article
- Kim YJ, Lee MH, Kim HJ, Lim G, Choi YS, Park NG, Kim KK, Lee WI: Formation of highly efficient dye-sensitized solar cells by hierarchical pore generation with nanoporous TiO2 spheres. Adv Mater 2009, 21: 3668–3673. 10.1002/adma.200900294View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.